An anchoring strategy leads to enhanced proton conductivity in a new metal‒organic framework
Lo, Tien H. N.; Nguyen, My V.; Tu, Thach N.; Inorganic Chemistry Frontiers 4 (2017) 1509–; doi:10.1039/C7QI00350A

data_4349758
_publ_section_title
;
 An anchoring strategy leads to enhanced proton conductivity in a new
 metal--organic framework
;
_journal_issue                   9
_journal_name_full               'Inorganic Chemistry Frontiers'
_journal_page_first              1509
_journal_paper_doi               10.1039/C7QI00350A
_journal_volume                  4
_journal_year                    2017
_chemical_formula_sum            'C24 H8 I0 N0 O22.12 S2 Zr3'
_chemical_formula_weight         988.00
_chemical_name_systematic        VNU-17
_space_group_crystal_system      tetragonal
_space_group_IT_number           87
_space_group_name_Hall           '-I 4'
_space_group_name_H-M_alt        'I 4/m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2017-03-29 deposited with the CCDC.
2017-07-17 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.7506(5)
_cell_length_b                   17.7506(5)
_cell_length_c                   22.4863(7)
_cell_measurement_reflns_used    2728
_cell_measurement_temperature    93(2)
_cell_measurement_theta_max      65.2399
_cell_measurement_theta_min      3.1463
_cell_volume                     7085.1(4)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      93(2)
_diffrn_detector_area_resol_mean 10.4167
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.3155
_diffrn_reflns_av_unetI/netI     0.1553
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            14660
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        62.348
_diffrn_reflns_theta_max         62.348
_diffrn_reflns_theta_min         3.172
_exptl_absorpt_coefficient_mu    4.501
_exptl_absorpt_correction_T_max  0.7523
_exptl_absorpt_correction_T_min  0.4808
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    0.926
_exptl_crystal_description       Needle
_exptl_crystal_F_000             1924
_exptl_crystal_recrystallization_method Solvothermal
_exptl_crystal_size_max          0.173
_exptl_crystal_size_mid          0.070
_exptl_crystal_size_min          0.068
_platon_squeeze_details
;
;
_refine_diff_density_max         1.574
_refine_diff_density_min         -3.316
_refine_diff_density_rms         0.253
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     132
_refine_ls_number_reflns         2910
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.060
_refine_ls_R_factor_all          0.1583
_refine_ls_R_factor_gt           0.1196
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1562P)^2^+223.7913P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2832
_refine_ls_wR_factor_ref         0.3062
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2159
_reflns_number_total             2910
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7qi00350a2.cif
_cod_data_source_block           VNU-17
_cod_original_cell_volume        7085.1(5)
_cod_database_code               4349758
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              32883
_shelx_hkl_checksum              11231